Admixture of an s-Wave Component to the d-Wave Gap
Symmetry in High-Temperature Superconductors
Received: 10 June 2007 / Accepted: 3 July 2007 / Published online: 3 August 2007 © Springer Science+Business Media, LLC 2007
Abstract Neutron crystal-field spectroscopy experiments in the Y- and La-type high-temperature superconductors HoBa2Cu3O6.56, HoBa2Cu4O8, and La1.81Sr0.15Ho0.04 -CuO4 are reviewed. By this bulk-sensitive technique, in-formation on the gap function is obtained from the relax-ation behavior of crystal-field transitions associated with the Ho3+ ions which sit as local probes close to the su-perconducting copper-oxide planes. The relaxation data ex-hibit a peculiar change from a convex to a concave shape between the superconducting transition temperature Tcand the pseudogap temperature T∗ which can only be modeled satisfactorily if the gap function of predominantly d-wave symmetry includes an s-wave component of the order of 20– 25%, independent of the doping level. Moreover, our results are compatible with an unusual temperature dependence of the gap function in the pseudogap region (Tc≤ T ≤ T∗), i.e., a break up of the Fermi surface into disconnected arcs. Keywords High-temperature superconductors· Gap symmetry· Pseudogap · Crystal field · Neutron spectroscopy
Ever since the discovery of high-temperature supercon-ductivity by Bednorz and Müller , there has been a debate concerning the symmetry of the superconducting gap function. So far, tunneling measurements are the only
A. Furrer ()
Laboratory for Neutron Scattering, ETH Zurich & PSI Villigen, CH-5232 Villigen PSI, Switzerland
phase-sensitive experiments that probe the sign of the order parameter . Angle-resolved photoemission spectroscopy (ARPES) measurements, on the other hand, yield very di-rect information about the magnitude and the momentum dependence of the order parameter as well as its evolution with temperature [3, 4]. Tunneling as well as ARPES ex-periments indicate that a dx2−y2 order parameter is the most
plausible candidate to describe the superconducting state in these systems. However, both techniques are only sensitive to the surface. As pointed out by Müller , the gap func-tion is different at the surface and in the bulk, thus bulk ex-periments are indispensable to unambiguously establish the nature of the gap function. Various experiments probing the bulk gave evidence for the existence of an s-wave compo-nent, but the results are partially conflicting. For optimally doped YBa2Cu3O7, e.g., Raman scattering evidences an s-wave admixture of 5% , thermal conductivity measure-ments in a rotating magnetic field place a maximum of 10% based on the shift of the nodal positions from the princi-pal diagonal directions , and nuclear magnetic resonance experiments report either an s-wave admixture of 20%  or a pure d-wave symmetry . Theoretical work based on the t–t–J model suggests that d-wave pairing prevails close to optimum doping, whereas s-wave-like pairing is possible in the under- and over-doped regimes . Doping-dependent bulk experiments are, therefore, extremely useful to shed light on this issue. The present work deals with such an investigation for underdoped and optimally doped
high-Tccompounds studied by neutron crystal-field spectroscopy experiments.
Neutron crystal-field spectroscopy is a powerful experi-mental tool to probe the bulk properties of high-temperature superconductors. It has been applied in the past mainly to detect the doping, isotope, and pressure dependence of the pseudogap temperature T∗. In principle, information on the
nature of the gap function can be obtained as well, pro-vided that the experimental data sets are sufficiently com-plete. We reviewed the available data sets in the literature and found the necessary conditions fulfilled for some un-derdoped and optimally doped La- and Y-based high-Tc compounds. We analyzed the corresponding data sets and found evidence for a 20–25% s-wave admixture to the dom-inant d-wave gap function, independent of the doping level. Moreover, our analysis supports the unusual temperature dependence of the gap function in the pseudogap region (Tc≤ T ≤ T∗) as evidenced by ARPES measurements in Bi2Sr2CaCu2O8+x.
2 Neutron Crystal-Field Spectroscopy
The principle of neutron crystal-field spectroscopic investi-gations of the crystal-field interaction in rare-earth based high-temperature superconductors was described in a re-cent review article . By this technique, transitions be-tween different crystal-field levels associated with the rare-earth ions can be directly measured. In the normal metallic state, the excited crystal-field levels interact with phonons, spin fluctuations and charge carriers, which limit the life-time of the excitation, thus the observed crystal-field tran-sitions exhibit line broadening. The interaction with the charge carriers is by far the dominating relaxation mecha-nism . The corresponding intrinsic linewidth Wn(T ) in-creases almost linearly with temperature according to the well-known Korringa law , i.e., Wn(T )∼ T . In the pseudogap as well as in the superconducting state, how-ever, the pairing of the charge carriers creates an energy gap
Δk in the single-electron spectral function (k is the wave vector), thus crystal-field excitations with energy <2Δkdo not have enough energy to span the gap. Consequently, the interaction with the charge carriers is suppressed, and for an isotropic gap function Δk = Δ, the intrinsic linewidth is given by Ws(T )= Wn(T )· exp[−Δ/kBT]. This means that Ws(T Tc, T∗)≈ 0, and line broad-ening sets in just below Tc (or T∗) where the supercon-ducting gap (or the pseudogap) opens. For anisotropic gap functions, the situation is more complicated, since cer-tain relaxation channels exist even at the lowest tempera-tures .
Recently, Häfliger et al.  presented detailed consid-erations concerning the analysis of neutron crystal-field re-laxation data with respect to the nature of the gap func-tion. As mentioned above, a crucial point in such analy-ses is the availability of a sufficient number of relax-ation data over a large temperature range, notably for the pseudogap region Tc≤ T ≤ T∗, so that the subtle but rel-evant features of the relaxation behavior can unambigu-ously be assessed. So far, such complete data sets are
Fig. 1 Temperature dependence of the intrinsic linewidth of the lowest crystal-field ground-state transition in HoBa2Cu3O6.56 (a),
HoBa2Cu418O8 (b), and La1.81Sr0.15Ho0.04Cu18O4(c). The dashed
line corresponds to the linewidth in the normal state as expected from the Korringa law
only available for underdoped HoBa2Cu3O6.56, slightly underdoped HoBa2Cu418O8 , and optimally doped La1.81Sr0.15Ho0.04Cu18O4  as shown in Figs.1(a–c). For all three compounds, the temperature dependence of the intrinsic linewidth W (T ) behaves in a common and charac-teristic way:
(i) T ≤ Tc: The linewidth is very small, but a slight en-hancement is observed upon approaching Tc.
(ii) T ≥ T∗: The linewidth increases linearly as expected for the normal state, so that we identify T∗ with the temperature where the pseudogap opens.
(iii) Tc ≤ T ≤ T∗: There is a sudden increase of the linewidth just above Tc. Then, with increasing tem-perature, the slope dW/dT is slightly reduced, but increases again upon approaching T∗. The
tempera-ture dependence of the linewidth obviously exhibits a change from a convex to a concave shape in the pseudo-gap region.
The only differences between the three data sets are the dif-ferent sizes of the characteristic temperatures Tcand T∗. It is, therefore, useful to express the relaxation data in reduced units, i.e., the temperature T in units of T∗and the linewidth
W (T )in units of W (T∗)as visualized for the relevant tem-perature range 0≤ T ≤ T∗in Figs.2(b–d).
3 Analysis of the Relaxation Data
We now proceed to analyze the relaxation data in terms of different gap functions. The model calculations were based on the procedure described in Ref. . For the tempera-ture dependence of the gap amplitude, we used the expres-sion Δ(T )= Δ(0) · [1 − (T /T∗)A] with A = 4 , and the maximum gap amplitude was set to Δmax/ kB= 2T∗
which is a realistic value for the compounds under consider-ation. Figure2(a) shows some calculations for an s-wave, a d-wave (dx2−y2), and a mixed (s25%+ d75%)-wave gap function. It can readily be seen that none of these mod-els is able to explain the observed linewidth behavior dis-played in Figs.2(b–d). The s-wave model reproduces the low-temperature behavior up to Tc quite well, but it fails completely at high temperatures. The d-wave model is inad-equate at both low and high temperatures. The mixed (s +d)-wave model has similar deficiencies. In particular, the be-havior around Tc where the slope of W (T )/W (T∗)turns from being convex to concave cannot be reproduced by any of the above models. This is due to the neglect of the tem-perature dependence of the gap function in the pseudogap region. According to ARPES experiments performed for un-derdoped Bi2Sr2CaCu2O8+x , the pseudogap opens up at different temperatures for different points in momentum space as sketched in Fig.3. Below T∗, there is a break up of the Fermi surface into disconnected arcs, which then shrink
Fig. 2 Temperature
dependence of the linewidth of low-energy crystal-field transitions in high-temperature superconductors in reduced units. (a) Model calculations for different types of gap functions (see text). (b–d) Relaxation data derived for HoBa2Cu3O6.56(b),
The lines in (b–d) denote least-squares fits on the basis of a mixed (s+ d)-wave gap function including the
occurrence of gapless arcs of the Fermi surface in the pseudogap region (Tc< T < T∗)as
described in the text
Fig. 3 Schematic illustration of the temperature evolution of the Fermi surface in the pseudogap region (Tc≤ T ≤ T∗). The
d-wave node below Tc(left
panel) becomes a gapless arc above Tc(middle panel) which
expands upon increasing the temperature to form the full Fermi surface at T∗(right panel)
Table 1 Gap parameters resulting from the least-squares fitting procedure applied to the crystal-field relaxation data displayed in Figs.2(b–d)
Tc[K] T∗[K] Δs[meV] Δd[meV] Δmax[meV]
HoBa2Cu3O6.56 60 250 8.6± 1.2 28.0± 2.1 36.6± 3.3
HoBa2Cu418O8 79 231 9.3± 0.9 28.5± 1.6 37.8± 2.5
La1.81Sr0.15Ho0.04Cu18O4 32 70 2.4± 0.4 7.7± 0.7 10.1± 1.1
with decreasing temperature before collapsing to the point nodes of the d-wave component below Tc. This unusual temperature evolution of the pseudogap opens additional re-laxation channels in crystal-field linewidth studies above Tc. Indeed, model calculations including the presence of such gapless arcs produce relevant modifications of the linewidth for Tc≤ T ≤ T∗as visualized in Fig.2(a); in particular, the observed change of the linewidth from a convex to a con-cave temperature dependence around Tc can be nicely re-produced for a mixed (s+ d)-wave gap function, but not for a pure d-wave gap function.
We performed a least-squares fitting procedure to the relaxation data displayed in Figs. 2(b–d) on the basis of a mixed (s+ d)-wave gap function including the gapless arc features of the Fermi surface in the pseudogap region
(Tc≤ T ≤ T∗). Since the latter effect was only observed at a few selected temperatures , we assumed a linear evolution of the gapless arcs with temperature. The only fit-ting parameters were the amplitudes Δs and Δd of the s-and d-wave components, respectively. The temperature evo-lution of the linewidths resulting from the least-squares fit-ting procedure are in good agreement with the experimen-tal data as shown in Figs.2(b–d). The corresponding model parameters are listed in Table 1. We recognize that the s-wave admixture is independent of the doping level, and the maximum gap amplitudes are consistent with the expecta-tion Δmax/ kB≈ 2T∗.
4 Concluding Remarks
In conclusion, our analyses of bulk-sensitive crystal-field relaxation experiments on high-temperature superconduc-tors give two important results. First, we gave evidence that the theoretically predicted  and for underdoped Bi2Sr2CaCu2O8+x observed  gapless arcs of the Fermi surface are also present in the Y- and La-based high-temperature superconductors, thereby being presumably a generic feature of all copper-oxide perovskites. Secondly, there is evidence for an admixture of an appreciable s-wave component of the order of 20–25% to the predom-inant d-wave gap function in both Y- and La-based
high-Tc superconductors. In fact, for orthorhombic symmetry both the s- and d-wave pair states belong to the same ir-reducible representation , thus an admixture of these
two states is allowed. Recent angle-resolved electron tun-neling experiments in YBa2Cu3O7 report similar results, namely a 17% s-wave admixture to the d-wave gap func-tion . Moreover, the gap values listed for the La-based compound in Table 1 are in good agreement with the results of recent in-plane magnetic-field penetration-depth measurements in La1.83Sr0.17CuO4 by muon-spin rotation experiments which gave Δs= 1.57(8) meV and
Δd= 8.2(1) meV . A subsequent theoretical study con-firmed these findings by calculations based on a two-band model .
Acknowledgement The author is very much indebted to K.A. Mü-ller for stimulating discussions.
1. Bednorz, J.G., Müller, K.A.: Z. Phys. B 64, 189 (1986) 2. Tsuei, C.C., Kirtley, J.R.: Rev. Mod. Phys. 72, 969 (2000) 3. Ding, H., Yokoya, T., Campuzano, J.C., Takahashi, T., Randeria,
M., Norman, M.R., Mochiku, T., Kadowaki, K., Giapintzakis, J.: Nature 382, 51 (1996)
4. Mesot, J., Norman, M.R., Ding, H., Randeria, M., Campuzano, J.C., Paramekanti, A., Fretwell, H.M., Kaminski, A., Takeuchi, T., Yokoya, T., Sato, T., Takahashi, T., Mochiku, T., Kadowaki, K.: Phys. Rev. Lett. 83, 840 (1999)
5. Müller, K.A.: Phil. Mag. Lett. 82, 279 (2002)
6. Limonov, M.F., Rykov, A.I., Tajima, S., Yamanaka, A.: Phys. Rev. Lett. 80, 825 (1998)
7. Aubin, H., Behnia, K., Ribault, M., Gagnon, R., Taillefer, L.: Phys. Rev. Lett. 78, 2624 (1997)
8. Stern, R., Mali, M., Roos, J., Brinkmann, D.: Phys. Rev. B 51, 15478 (1995)
9. Bulut, N., Scalapino, D.J.: Phys. Rev. Lett. 67, 2898 (1991) 10. Wheatley, J., Xiang, T.: Solid State Commun. 88, 593 (1993) 11. Norman, M.R., Ding, H., Randeria, M., Campuzano, J.C., Yokoya,
T., Takeuchi, T., Takahashi, T., Mochiku, T., Kadowaki, K., Gup-tasarma, P., Hinks, D.G.: Nature 392, 157 (1998)
12. Furrer, A.: Struct. Bond. 114, 171 (2005) 13. Boothroyd, A.T.: Phys. Rev. B 64, 066501 (2001) 14. Korringa, J.: Physica (Utrecht) 16, 601 (1950)
15. Boothroyd, A.T., Mukherjee, A., Murani, A.P.: Phys. Rev. Lett. 77, 1600 (1996)
16. Häfliger, P.S., Podlesnyak, A., Conder, K., Pomjakushina, E., Fur-rer, A.: Phys. Rev. B 74, 184520 (2006)
17. Rubio Temprano, D., Mesot, J., Conder, K., Janssen, S., Mutka, H., Furrer, A.: J. Supercond. 13, 727 (2000)
18. Rubio Temprano, D., Mesot, J., Janssen, S., Conder, K., Furrer, A., Mutka, H., Müller, K.A.: Phys. Rev. Lett. 84, 1990 (2000) 19. Rubio Temprano, D., Conder, K., Furrer, A., Mutka, H., Trounov,
V., Müller, K.A.: Phys. Rev. B 66, 184506 (2002) 20. Wen, X.G., Lee, P.A.: Phys. Rev. Lett. 76, 503 (1996)
21. Annett, J.F., Goldenfeld, N.D., Renn, S.R.: In: Ginsberg, D.M. (ed.) Physical Properties of High-Temperature Superconductors II, p. 571. World Scientific, Singapore (1990)
22. Smilde, H.J.H., Golubov, A.A., Ariando, G., Rijnders, G., Dekkers, J.M., Harkema, S., Blank, D.H.A., Rogalla, H., Hilgenkamp, H.: Phys. Rev. Lett. 95, 257001 (2005)
23. Khasanov, R., Shengelaya, A., Maiuradze, A., La Mattina, F., Bussmann-Holder, A., Keller, H., Müller, K.A.: Phys. Rev. Lett. 98, 057007 (2007)
24. Bussmann-Holder, A., Khasanov, R., Shengelaya, A., Maisuradze, A., La Mattina, F., Keller, H., Müller, K.A.: Europhys. Lett. 77, 27002 (2007)